Plane Strain Test for Metal Sheet Characterization


 Terence Stevenson
 1 years ago
 Views:
Transcription
1 Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue du Président Wilson 62, Cachan Cedex, France 3 Department of ArGEnCO, University of Liège, Chemin des Chevreuils 1, B4000 Liège, Belgium Abstract This article shows the influence of a plane strain test specimen geometry on the measurable strain field and the influence of free edge effects over the stress computation. The experimental strain field distribution is measured over the whole deformable zone of a plane strain test specimen by an optical strain gauge. The chosen material is the DC06 IF steel of 0.8 mm thickness. The stress field is computed for several geometries at different strain levels by a Finite Element (FE) commercial code (Samcef ). The results show that the stress field is sensitive to the specimen's geometry and also to the tested material (strain field behavior is independent of material) and, based on results, an optimal specimen geometry is proposed in order to minimized the stress computation error. Keywords: Material characterization, mechanical tests, stress  strain field homogeneity. Introduction Industrial requirements for lighter components and structures have motivated the study of material behavior in order to save manufacturing and transportation energy. Different metal forming processes such as deep drawing, bending or stamping are required to manufacture automotive parts or beverage cans. The finite element method (FEM) is quite successful to simulate those metal forming processes, but accuracy depends both on the constitutive laws used and their material parameters identification. Constitutive models for sheet metal forming at room temperature include a yield surface defined by a yield criterion, a normality rule and a hardening law (yield surface evolution). Accurate phenomenological yield criteria are defined by material parameters that must be identified by several mechanical tests such as uniaxial tensile test, equibiaxial test, biaxial test, plane strain test and simple shear test. The goal of this work is to define a plane strain test specimen geometry in which the stress and the strain tensor fields have a quasihomogeneous behavior. A homogeneous behavior of those tensor fields allows the computation of the stress state directly from the force and deformation data and simplifies the parameters identification routines. The stress  strain state of the plane strain test and the experimental set up is described in next section. A strategy using FEM to study the stress field homogeneity is proposed in section 2. The results are discussed in section 3 and finally some conclusions are established and some perspectives proposed. Regarding notation, lowercase boldface Latin letters are used for vectors and uppercase boldface letters (Latin or Greek) to define second order tensor. The tensor product is defined by Description of the Plane Strain Test The plane strain test reproduces a particular case of the plane stress state in which one of the principal strain values and the shear components equal zero. This test is widely used in material characterization (yield surface and work hardening) and to obtain forming limits diagrams.
2 Mechanical Conditions Fig. 1 sketches the axis over a laminated sheet. The material axes defined by the rolling direction (RD), the transversal direction (TD) and the normal direction (ND) are coincident with the X 1, X 2 and X 3 axes. Assuming a plane stress state, the second order Cauchy stress tensor can be defined as follows: Figure 1: Rolled sheet axis definition, α defines the angle with respect to the RD. To represent the stress state for any angle a the following transformation linking a state defined in the x 1, x 2 and x 3 axes with the X 1, X 2 and X 3 is used: where R is a proper orthogonal second order tensor (i.e. R T R = RR T = I and det R = 1) defined by Then, the general expression for the plane stress state is defined as follows: The principal stretches of the sheet are represented by λ i (i = 1, 2, 3) in the second order stretch tensor U: The logarithmic strain is defined in terms of the principal stretches as: For the plane strain case λ 2 = 1, then ε 2 = 0. Assuming volume conservation, i.e., λ 1 λ 2 λ 3 = 1 (or ε 1 + ε 2 + ε 3 = 0), the logarithmic strain tensor components are related by ε 1 = ε 3.
3 In plasticity, the plastic strain rate tensor is related to the Cauchy stress tensor by the normality rule: where is the plastic multiplier and is the plastic potential function represented, in this work, by the Hill 1948 orthotropic yield criterion [1]: H, G, F, N, M, L are material parameters and k(p) describes the yield surface size evolution (isotropic hardening) in terms of the equivalent plastic strain. Using the condition ε 2 = 0 one can assume that: which allows the representation of one component of the Cauchy stress tensor in terms of the other (Eq. 10). This has particular significance when the stress data is used to identify yield function material parameters (e.g. when using the "plastic contours method" [2,3]) since most of the testing machines do not count with a proper device to measure the stress component in perpendicular direction with respect to the applied load. Eq. 10 can be seen as a generalization of the isotropic case when k a = 0,5. The relation shown in Eq. 10 can be obtained for other yield criteria as it is shown in [4]. Experimental set up Fig. 2a shows the biaxial testing machine built at the ArGEnCO Laboratory at the University of Liege [5]. The arrows in the figure show the machine movement axes. The motion is generated by two hydraulic pistons, which can be controlled in displacement or force simultaneously or independently. These motions enable us to perform simple shear and plane strain tests. Fig. 2b shows a detail of the specimen's measurable zone clamped by hydraulics grips. The specimen geometry designed for the biaxial testing machine is shown in Fig. 3a where the dotted area is the measurable zone. The deformation is imposed by the pistons (vertical for the plane strain test and horizontal for the simple shear test) of the biaxial testing machine. The strain field can be measured in the whole deformation zone (due to an optical strain gauge), and the average stress σ 11 is computed form the load cell data and the actual area as it is shown in Fig. 3b. This assumption is only valid if the stress field is homogeneous. The component σ 22 of the stress tensor cannot be measured with this mechanical configuration.
4 Figure 2: Biaxial testing machine designed at the ArGEnCO Laboratory, University of Liege. Figure 3: (a) Specimen geometry and deformation area, (b) Sketch of the stress distribution. Fig. 4 shows the experimental strain field distribution at the centerline level (Fig. 3b) for the logarithmic strain tensor components ε 11 and ε 22. The test is done over a DC06 IF steel of 0.8mm thickness (anyways, the strain distribution is independent of the material). The following conclusions can be drawn from these results: the strain tensor is homogeneous over the deformation area except at the free edges, the homogeneity depends on the amount of the imposed deformation (ε 11 ), the strain component ε 22 is negligible in the homogeneous zone of the deformation area and, by volume conservation, the condition ε 1 = ε 3 is valid over the homogeneous zone of the deformation area. These conclusions are valid for the specimen geometry of Fig. 4a, i.e., when h/b=10. The influence of deformation area geometry, the imposed strain level and the material over the stress field is studied in what follows by a FE simulation of the plane strain test.
5 Figure 4: (a) ε 11 strain distribution over the specimen centerline, (b) ε 22 strain distribution over the specimen centerline. Figure 5: Stress field in the loading direction for ε 11 = 20%, h/b=20 and thickness t=1.5mm.
6 Plane Strain Test FE Simulation The FE simulation of the test is used to study the stress field distribution over the deformable zone of the specimen. By studying the influence of the edge effect over several geometries, the obtained results help to define a criterion to define whether a stress field can be consider (quasi)homogeneous or heterogeneous. Simulation Parameters The simulation parameters appear in Table 1 and only the deformation area is simulated (sliding of the specimen inside the grips is neglected), the used mesh appears in Fig. 5. To study the influence of the material in the stress field, the results obtained out of two materials are compared. Material 1 corresponds to the IF steel DC06 characterized in [3,5], Material 2 is a Active material that has the same initial yield locus as Material 1, but a different hardening behavior (hardening stagnates at 10% of deformation). The initial yield locus material parameters for the Hill 1948 criterion (Eq. 8) are in Table 2 and Table 3 contains the hardening parameters. The elastic modulus is E = [MPa] and Poisson's coefficient v=0.3. Table 1: Finite element strategy. Code Element Type Finite Element Simulation Data Integration Points 8 Number of Elements Constitutive Law Samcef v1 1.1 (Samtech) Brick 5400 (3 thickness layers) Elastoplastic Hill 1948 coupled with isotropic hardening Table 2: Initial yield surface material parameters for Hill 1948 criterion. DC06 0.8mm Material Parameters for Hill 1948 criterion H F G N M L [MPa] Table 3: Hardening laws material parameters. Hardening Law Material Parameters for Hardening Laws Material Parameters Material 1 K [MPa] ε 0 n (DC06 0.8mm) k(p)=k(ε 0 +p) n Material 2 k(p) = σ y + R SAT [1exp(C R p)] σ y [MPa] R SAT [MPa] C R Comparing Variables The average stress is defined by Eq. 11, here V i represents the volume of the element, V total the total volume of the deformable area and σ i is the stress value of the element (in the loading direction). This stress computation is impossible to obtain experimentally. A second stress definition is given by Eq. 12. F is the load measured by the load cell and A CL is the cross section area computed at the centerline of the specimen's deformation area. In this case, the stress value can be obtained
7 experimentally but it involves expensive equipment and it is time consuming. A third definition is presented in Eq. 13. F is the load measured by the load cell and A CP is the cross section area computed with the information obtained at the center point of the specimen's deformation area. Assuming volume conservation in plasticity, this cross section area can be obtained from Eq. 14, where A 0 is the initial cross section area of the specimen and ε CP 11 is the strain measured in the load direction at the center point of the deformation area. Then, in order to define a homogeneity criterion, the stress values obtained from Eq. 12 and 13 are compared with the one given for Eq. 11 for a quasihomogeneous, arbitrary chosen, stress distribution. This reference stress is obtained from a geometrical ratio of h/b=20 (a higher ratio would not be economically viable) and t=1.5mm since the absolute relative error between σ global (or σ true ) and σ ave is not greater than 0.5% for an imposed strain of 20% for Material 1 (see Fig. 5) and 10% for Material 2. Results Fig. 6 shows the error at different strain levels for different specimen's geometries. It is clear that increasing the ratio h/b, the error between the average stress (taken as a reference value) and the global and true stress diminish. The influence of the strain level does not seem to have a large influence on the error evolution. The error obtained by using the true stress definition is less than 0.2% in the most adverse case (h/b=5) when comparing with the error given by the global stress definition, this means that for a ratio higher than h/b=10 the actual area can be obtained from measures taken at the center of the specimen (Eq. 14), saving important data processing time. Fig. 7 shows that the stress error depends on the material (unlike the strain fields), hence it makes impossible to compute a general correction factor. Fig. 8 shows that homogeneity also depends (slightly) on the specimen's thickness.
8 Figure 6: Stress error in terms of h/b for Material 1, (a) for σ global, (b) for σ true.
9 Figure 7: Differences of the stress error depending on the material, (a) for σ giobai, (b) for σ true.
10 Figure 8: Influence of the thickness specimen in the error.
11 Figure 9: Modifications at the free edge levels of the specimen.
12 Conclusions and Perspectives The geometrical ratio h/b=10 in the measurable zone of the specimen geometry seems to be the most performing since the stress error is less than 1% for the two materials. It also ensures that the strain in the sense perpendicular to the impose deformation ε 22 remains negligible during the deformation process. The actual area can be measured from the center point data. The thickness variation does not seem to contribute significantly to the stress error. Even if the final stress error could be quantified, this has not practical interest since the stress field is dependent on the material; hence it is impossible to define a general correction factor. From this work another criterion of homogeneity can be proposed in order to neglect the component ε 22 in the strain tensor: the strain average taken over an 80% of central part of the deformation area must by much lower than the one measure at the free edges (as observed in Fig. 4b). In this case, it is necessary to compute the whole strain field. In future, the specimen geometry will be slightly modified at the free edge level (Fig. 9) in order to study the failure position which occurs near the free edges, where strain and stress concentrations are higher as it is shown respectively in Fig. 4 and Fig. 5. Acknowledgement As Research Director, AnneMarie Habraken would like to thank the National Found for Scientific Research (FNRS, Belgium) for its support. References [1] R. Hill: The Mathematical Theory of Plasticity (The Oxford Eng Sciences Series, 1950). [2] T. Kuwabara, A. Van Beal, E. Iizuka: Acta Materialia Vol. 50 (2002), pp [3] P. Flores, P. Moureaux, A.M. Habraken: Material Identification using a Biaxial Test Machine (Trans Tech Publications, Switzerland 2005). [4] P. Flores: Development of Experimental Equipment and Identification Procedures for Sheet Metal Constitutive Laws (PhD Thesis, University of Liege  Belgium, 2005). [5] P. Flores, E. Rondia, A.M. Habraken: International Journal of Forming Processes, Special Issue (2005) pp
Enhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationA ratedependent HosfordCoulomb model for predicting ductile fracture at high strain rates
EPJ Web of Conferences 94, 01080 (2015) DOI: 10.1051/epjconf/20159401080 c Owned by the authors, published by EDP Sciences, 2015 A ratedependent HosfordCoulomb model for predicting ductile fracture at
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationANALYSIS AND NUMERICAL MODELLING OF CERAMIC PIEZOELECTRIC BEAM BEHAVIOR UNDER THE EFFECT OF EXTERNAL SOLICITATIONS
Third International Conference on Energy, Materials, Applied Energetics and Pollution. ICEMAEP016, October 3031, 016, Constantine,Algeria. ANALYSIS AND NUMERICAL MODELLING OF CERAMIC PIEZOELECTRIC BEAM
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationConstitutive models: Incremental plasticity Drücker s postulate
Constitutive models: Incremental plasticity Drücker s postulate if consistency condition associated plastic law, associated plasticity  plastic flow law associated with the limit (loading) surface Prager
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationStructural Metals Lab 1.2. Torsion Testing of Structural Metals. Standards ASTM E143: Shear Modulus at Room Temperature
Torsion Testing of Structural Metals Standards ASTM E143: Shear Modulus at Room Temperature Purpose To determine the shear modulus of structural metals Equipment TiniusOlsen LoTorq Torsion Machine (figure
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 LABORATORY ASSIGNMENT NUMBER 6
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 LABORATORY ASSIGNMENT NUMBER 6 COMPRESSION TESTING AND ANISOTROPY OF WOOD Purpose: Reading: During this laboratory
More informationAnalytical and experimental evaluation of the stressstrain curves of sheet metals by hydraulic bulge tests
Analytical and experimental evaluation of the stressstrain curves of sheet metals by hydraulic bulge tests Lucian LĂZĂRESCU 1, a, DanSorin COMŞA 1,b and Dorel BANABIC 1,c 1 Technical University of ClujNapoca,
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationTransactions on Modelling and Simulation vol 10, 1995 WIT Press, ISSN X
Parameters controlling the numerical simulation validity of damageable composite toughness testing S. Yotte, C. Currit, E. Lacoste, J.M. Quenisset Laboratoire de Genie Meanique  IUT 'A\ Domaine Universitaire,
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationComputational models of diamond anvil cell compression
UDC 519.6 Computational models of diamond anvil cell compression A. I. Kondrat yev Independent Researcher, 5944 St. Alban Road, Pensacola, Florida 32503, USA Abstract. Diamond anvil cells (DAC) are extensively
More informationPullout Tests of Geogrids Embedded in Noncohesive Soil
Archives of HydroEngineering and Environmental Mechanics Vol. 51 (2004), No. 2, pp. 135 147 Pullout Tests of Geogrids Embedded in Noncohesive Soil Angelika Duszyńska, Adam F. Bolt Gdansk University of
More informationScienceDirect. Bauschinger effect during unloading of coldrolled copper alloy sheet and its influence on springback deformation after Ubending
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 81 (2014 ) 969 974 11th International Conference on Technology of Plasticity, ICTP 2014, 1924 October 2014, Nagoya Congress
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationDetermination of stressstrain curves of sheet metals by hydraulic bulge test
Determination of stressstrain curves of sheet metals by hydraulic bulge test Lucian LĂZĂESCU, Dan Sorin COMŞA and Dorel BANABIC Technical University of ClujNapoca, Department of Manufacturing Engineering,
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationINVERSE METHOD FOR FLOW STRESS PARAMETERS IDENTIFICATION OF TUBE BULGE HYDROFORMING CONSIDERING ANISOTROPY
7 th EUROMECH Solid Mechanics Conference J. Ambrósio et.al. (eds.) Lisbon, Portugal, September 711, 2009 INVERSE METHOD FOR FLOW STRESS PARAMETERS IDENTIFICATION OF TUBE BULGE HYDROFORMING CONSIDERING
More information6.37 Determine the modulus of resilience for each of the following alloys:
6.37 Determine the modulus of resilience for each of the following alloys: Yield Strength Material MPa psi Steel alloy 550 80,000 Brass alloy 350 50,750 Aluminum alloy 50 36,50 Titanium alloy 800 116,000
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationThe design of a formula student front impact attenuator
The design of a formula student front impact attenuator J.M.J. Schormans MT 10.06 Supervisors: dr. ir. Varvara Kouznetsova Eindhoven University of Technology Department of Mechanical Engineering Computational
More informationConcept Question Comment on the general features of the stressstrain response under this loading condition for both types of materials
Module 5 Material failure Learning Objectives review the basic characteristics of the uniaxial stressstrain curves of ductile and brittle materials understand the need to develop failure criteria for
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More information14. LSDYNA Forum 2016
14. LSDYNA Forum 2016 A Novel Approach to Model Laminated Glass R. Böhm, A. Haufe, A. Erhart DYNAmore GmbH Stuttgart 1 Content Introduction and Motivation Common approach to model laminated glass New
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationLecture 8 Viscoelasticity and Deformation
HW#5 Due 2/13 (Friday) Lab #1 Due 2/18 (Next Wednesday) For Friday Read: pg 130 168 (rest of Chpt. 4) 1 Poisson s Ratio, μ (pg. 115) Ratio of the strain in the direction perpendicular to the applied force
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationNumerical and Experimental Studies on Thermoforming Process. Sogang University
Numerical and Experimental Studies on Thermoforming Process Thermoforming Process Hot plate Atmosphere Seal Mold Air on Air on Vacuum or atmosphere Introduction Thermoforming Process Advantage Low forming
More informationIdentification of the plastic zone using digital image correlation
M. Rossi et alii, Frattura ed Integrità Strutturale, 3 (4) 55557; DOI:.3/IGFESIS.3.66 Focussed on: Fracture and Structural Integrity related Issues Identification of the plastic zone using digital image
More informationStress, Strain, Mohr s Circle
Stress, Strain, Mohr s Circle The fundamental quantities in solid mechanics are stresses and strains. In accordance with the continuum mechanics assumption, the molecular structure of materials is neglected
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationAnalysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method
Analysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method V.M.F. Nascimento Departameto de ngenharia Mecânica TM, UFF, Rio de Janeiro
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationBrittle Deformation. Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm
Lecture 6 Brittle Deformation Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm WW Norton, unless noted otherwise Brittle deformation EarthStructure (2 nd
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationNumerical simulation the bottom structures. grounding test by LSDYNA
5 th European LSDYNA Users Conference Methods and Techniques (3) Numerical simulation the bottom structures grounding test by LSDYNA Ainian Zhang Graduate School of Frontier Sciences, The University
More informationFinite Element Modeling of an Aluminum Tricycle Frame
Finite Element Modeling of an Aluminum Tricycle Frame A. Rodríguez, B. Chiné*, and J. A. Ramírez Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationMODELING OF ELASTOPLASTIC MATERIALS IN FINITE ELEMENT METHOD
MODELING OF ELASTOPLASTIC MATERIALS IN FINITE ELEMENT METHOD Andrzej Skrzat, Rzeszow University of Technology, Powst. Warszawy 8, Rzeszow, Poland Abstract: Userdefined material models which can be used
More informationTesting and Analysis
Testing and Analysis Testing Elastomers for Hyperelastic Material Models in Finite Element Analysis 2.6 2.4 2.2 2.0 1.8 1.6 1.4 Biaxial Extension Simple Tension Figure 1, A Typical Final Data Set for Input
More informationLateral Earth Pressure
1 of 11 6/2/2012 4:28 AM Lateral Earth Pressure The magnitude of lateral earth pressure depends on: 1. Shear strength characteristics of soil 2. Lateral strain condition 3. Pore water pressure 4. State
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More informationInitial Stress Calculations
Initial Stress Calculations The following are the initial hand stress calculations conducted during the early stages of the design process. Therefore, some of the material properties as well as dimensions
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationEffect of Strain Hardening on Unloading of a Deformable Sphere Loaded against a Rigid Flat A Finite Element Study
Effect of Strain Hardening on Unloading of a Deformable Sphere Loaded against a Rigid Flat A Finite Element Study Biplab Chatterjee, Prasanta Sahoo 1 Department of Mechanical Engineering, Jadavpur University
More informationNumerical modelling of elasticplastic deformation at crack tips in composite material under stress wave loading
JOURNAL DE PHYSIQUE IV Colloque C8, supplément au Journal de Physique III, Volume 4, septembre 1994 C853 Numerical modelling of elasticplastic deformation at crack tips in composite material under stress
More informationCHAPTER OBJECTIVES CHAPTER OUTLINE. 4. Axial Load
CHAPTER OBJECTIVES Determine deformation of axially loaded members Develop a method to find support reactions when it cannot be determined from euilibrium euations Analyze the effects of thermal stress
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More informationAdvanced Friction Modeling in Sheet Metal Forming
Advanced Friction Modeling in Sheet Metal Forming J.Hol 1,a, M.V. Cid Alfaro 2, T. Meinders 3, J. Huétink 3 1 Materials innovation institute (M2i), P.O. box 58, 26 GA Delft, The Netherlands 2 Tata Steel
More informationA Finite Element Model for Numerical Analysis of Sintering
A Finite Element Model for Numerical Analysis of Sintering DANIELA CÂRSTEA HighSchool Group of Railways, Craiova ION CÂRSTEA Department of Computer Engineering and Communication University of Craiova
More informationFormulation of Equivalent Steel Section for Partially Encased Composite Column under Concentric Gravity Loading
Formulation of Equivalent Steel Section for Partially Encased Composite Column under Concentric Gravity Loading Debaroti Ghosh & Mahbuba Begum Dept of Civil Engineering, Bangladesh University of Engineering
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationBulk Metal Forming II
Bulk Metal Forming II Simulation Techniques in Manufacturing Technology Lecture 2 Laboratory for Machine Tools and Production Engineering Chair of Manufacturing Technology Prof. Dr.Ing. Dr.Ing. E.h.
More informationTHEME A. Analysis of the elastic behaviour of La Aceña archgravity dam
THEME A Analysis of the elastic behaviour of La Aceña archgravity dam Gjorgi KOKALANOV, Professor, Faculty of Civil Eng., Skopje, Republic of Macedonia Ljubomir TANČEV, Professor, Faculty of Civil Eng.,
More informationCurvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment. P. Krulevitch G. C. Johnson
UCRLJC30440 PREPRINT Curvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment P. Krulevitch G. C. Johnson This paper was prepared for submittal to the Materials Research Society Spring
More informationThe Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
11th European Conference on NonDestructive Testing (ECNDT 214), October 61, 214, Prague, Czech Republic The Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
More informationINFLUENCE OF WEB THICKNESS REDUCTION IN THE SHEAR RESISTANCE OF NONPRISMATIC TAPERED PLATE GIRDERS
INFLUENCE OF WEB THICKNESS REDUCTION IN THE SHEAR RESISTANCE OF NONPRISMATIC TAPERED PLATE GIRDERS Paulo J. S. Cruz 1, Lúcio Lourenço 1, Hélder Quintela 2 and Manuel F. Santos 2 1 Department of Civil
More informationAnisotropy and Failure Modeling for Nonlinear Strain. Paths and Its Application to Rigid Packaging. Robert Earl Dick (B.S.C.E, M.S.C.
Anisotropy and Failure Modeling for Nonlinear Strain Paths and Its Application to Rigid Packaging by Robert Earl Dick (B.S.C.E, M.S.C.E) Advisor: Jeong Whan Yoon Submitted in fulfillment of the requirements
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationAN IMPORTANT PITFALL OF PSEUDOSTATIC FINITE ELEMENT ANALYSIS
AN IMPORTANT PITFALL OF PSEUDOSTATIC FINITE ELEMENT ANALYSIS S. Kontoe, L. Pelecanos & D.M. Potts ABSTRACT: Finite Element (FE) pseudostatic analysis can provide a good compromise between simplified
More informationVibration analysis of free isotropic cracked plates
Computational Methods and Experimental Measurements XII 475 Vibration analysis of free isotropic cracked plates M. Alfano & L. Pagnotta Department of Mechanical Engineering, University of Calabria, Italy
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationTHE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE
Journal of Applied Mathematics and Computational Mechanics 013, 1(4), 131 THE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE Jolanta Błaszczuk
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationChapter 5 Torsion STRUCTURAL MECHANICS: CE203. Notes are based on Mechanics of Materials: by R. C. Hibbeler, 7th Edition, Pearson
STRUCTURAL MECHANICS: CE203 Chapter 5 Torsion Notes are based on Mechanics of Materials: by R. C. Hibbeler, 7th Edition, Pearson Dr B. Achour & Dr Eng. K. Elkashif Civil Engineering Department, University
More informationFRACTURE MECHANICS FOR MEMBRANES
FRACTURE MECHANICS FOR MEMBRANES Chong Li, Rogelio Espinosa and Per Ståhle Solid Mechanics, Malmö University SE 205 06 Malmö, Sweden chong.li@ts.mah.se Abstract During fracture of membranes loading often
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationMaterial removal, correction and laboratory Xray diffraction
Advanced Materials Research Online: 20140811 ISSN: 16628985, Vol. 996, pp 181186 doi:10.4028/www.scientific.net/amr.996.181 2014 Trans Tech Publications, Switzerland Material removal, correction and
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More information1.5 STRESSPATH METHOD OF SETTLEMENT CALCULATION 1.5 STRESSPATH METHOD OF SETTLEMENT CALCULATION
Module 6 Lecture 40 Evaluation of Soil Settlement  6 Topics 1.5 STRESSPATH METHOD OF SETTLEMENT CALCULATION 1.5.1 Definition of Stress Path 1.5. Stress and Strain Path for Consolidated Undrained Undrained
More informationModelling the excavation damaged zone in CallovoOxfordian claystone with strain localisation
Modelling the excavation damaged zone in CallovoOxfordian claystone with strain localisation B. Pardoen  F. Collin  S. Levasseur  R. Charlier Université de Liège ArGEnCo ALERT Workshop 2012 Aussois,
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More information(MPa) compute (a) The traction vector acting on an internal material plane with normal n ( e1 e
EN10: Continuum Mechanics Homework : Kinetics Due 1:00 noon Friday February 4th School of Engineering Brown University 1. For the Cauchy stress tensor with components 100 5 50 0 00 (MPa) compute (a) The
More informationPLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile
More information*MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials
14 th International LSDYNA Users Conference Session: Constitutive Modeling *MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials Jesper Karlsson 1, Mikael Schill 1, Johan Tryding
More informationFinite element simulation of residual stresses in laser heating
IAS200866546ST Finite element simulation of residual stresses in laser heating G. H. Farrahi 1, M. Sistaninia 2, H. Moeinoddini 3 1,2School of Mechanical Engineering, Sharif University of Technology,
More information